Upcoming SlideShare
×

# Axial deformation

2,688 views
2,567 views

Published on

1 Comment
1 Like
Statistics
Notes
• Full Name
Comment goes here.

Are you sure you want to Yes No
• its a very good book

Are you sure you want to  Yes  No
Views
Total views
2,688
On SlideShare
0
From Embeds
0
Number of Embeds
5
Actions
Shares
0
78
1
Likes
1
Embeds 0
No embeds

No notes for slide

### Axial deformation

1. 1. Strength of Materials Prof. M. S. Sivakumar Axial Deformations Introduction Free body diagram - Revisited Normal, shear and bearing stress Stress on inclined planes under axial loading Strain Mechanical properties of materials True stress and true strain Poissons ratio Elasticity and Plasticity Creep and fatigue Deformation in axially loaded members Statically indeterminate problems Thermal effect Design considerations Strain energy Impact loadingIndian Institute of Technology Madras
2. 2. Strength of Materials Prof. M. S. Sivakumar 1.1 Introduction An important aspect of the analysis and design of structures relates to the deformations caused by the loads applied to a structure. Clearly it is important to avoid deformations so large that they may prevent the structure from fulfilling the purpose for which it is intended. But the analysis of deformations may also help us in the determination of stresses. It is not always possible to determine the forces in the members of a structure by applying only the principle of statics. This is because statics is based on the assumption of undeformable, rigid structures. By considering engineering structures as deformable and analyzing the deformations in their various members, it will be possible to compute forces which are statically indeterminate. Also the distribution of stresses in a given member is indeterminate, even when the force in that member is known. To determine the actual distribution of stresses within a member, it is necessary to analyze the deformations which take place in that member. This chapter deals with the deformations of a structural member such as a rod, bar or a plate under axial loading. TopIndian Institute of Technology Madras
3. 3. Strength of Materials Prof. M. S. Sivakumar 1.2 Free body diagram - Revisited The first step towards solving an engineering problem is drawing the free body diagram of the element/structure considered. Removing an existing force or including a wrong force on the free body will badly affect the equilibrium conditions, and hence, the analysis. In view of this, some important points in drawing the free body diagram are discussed below. Figure 1.1 At the beginning, a clear decision is to be made by the analyst on the choice of the body to be considered for free body diagram. Then that body is detached from all of its surrounding members including ground and only their forces on the free body are represented. The weight of the body and other external body forces like centrifugal, inertia, etc., should also be included in the diagram and they are assumed to act at the centre of gravity of the body. When a structure involving many elements is considered for free body diagram, the forces acting in between the elements should not be brought into the diagram. The known forces acting on the body should be represented with proper magnitude and direction. If the direction of unknown forces like reactions can be decided, they should be indicated clearly in the diagram.Indian Institute of Technology Madras
4. 4. Strength of Materials Prof. M. S. Sivakumar After completing free body diagram, equilibrium equations from statics in terms of forces and moments are applied and solved for the unknowns. TopIndian Institute of Technology Madras
5. 5. Strength of Materials Prof. M. S. Sivakumar 1.3 Normal, shear and bearing stress 1.3.1 Normal Stress: Figure 1.2 When a structural member is under load, predicting its ability to withstand that load is not possible merely from the reaction force in the member. It depends upon the internal force, cross sectional area of the element and its material properties. Thus, a quantity that gives the ratio of the internal force to the cross sectional area will define the ability of the material in with standing the loads in a better way. That quantity, i.e., the intensity of force distributed over the given area or simply the force per unit area is called the stress. P σ= 1.1 A In SI units, force is expressed in newtons (N) and area in square meters. Consequently, the stress has units of newtons per square meter (N/m2) or Pascals (Pa). In figure 1.2, the stresses are acting normal to the section XX that is perpendicular to the axis of the bar. These stresses are called normal stresses. The stress defined in equation 1.1 is obtained by dividing the force by the cross sectional area and hence it represents the average value of the stress over the entire cross section.Indian Institute of Technology Madras
6. 6. Strength of Materials Prof. M. S. Sivakumar Figure 1.3 Consider a small area ∆A on the cross section with the force acting on it ∆F as shown in figure 1.3. Let the area contain a point C. Now, the stress at the point C can be defined as, ∆F σ = lim 1.2 ∆ A → 0 ∆A The average stress values obtained using equation 1.1 and the stress value at a point from equation 1.2 may not be the same for all cross sections and for all loading conditions. 1.3.2 Saint - Venants Principle: Figure 1.4Indian Institute of Technology Madras
7. 7. Strength of Materials Prof. M. S. Sivakumar Consider a slender bar with point loads at its ends as shown in figure 1.4. The normal stress distribution across sections located at distances b/4 and b from one and of the bar is represented in the figure. It is found from figure 1.4 that the stress varies appreciably across the cross section in the immediate vicinity of the application of loads. The points very near the application of the loads experience a larger stress value whereas, the points far away from it on the same section has lower stress value. The variation of stress across the cross section is negligible when the section considered is far away, about equal to the width of the bar, from the application of point loads. Thus, except in the immediate vicinity of the points where the load is applied, the stress distribution may be assumed to be uniform and is independent of the mode of application of loads. This principle is called Saint-Venants principle. 1.3.3 Shear Stress: The stresses acting perpendicular to the surfaces considered are normal stresses and were discussed in the preceding section. Now consider a bolted connection in which two plates are connected by a bolt with cross section A as shown in figure 1.5. Figure 1.5 The tensile loads applied on the plates will tend to shear the bolt at the section AA. Hence, it can be easily concluded from the free body diagram of the bolt that the internal resistance force V must act in the plane of the section AA and it should be equal to the external load P. These internal forces are called shear forces and when they are divided by the corresponding section area, we obtain the shear stress on that section.Indian Institute of Technology Madras
8. 8. Strength of Materials Prof. M. S. Sivakumar V τ= 1.3 A Equation 1.3 defines the average value of the shear stress on the cross section and the distribution of them over the area is not uniform. In general, the shear stress is found to be maximum at the centre and zero at certain locations on the edge. This will be dealt in detail in shear stresses in beams (module 6). In figure 1.5, the bolt experiences shear stresses on a single plane in its body and hence it is said to be under single shear. Figure 1.6 In figure 1.6, the bolt experiences shear on two sections AA and BB. Hence, the bolt is said to be under double shear and the shear stress on each section is V P τ= = 1.4 A 2A Assuming that the same bolt is used in the assembly as shown in figure 1.5 and 1.6 and the same load P is applied on the plates, we can conclude that the shear stress is reduced by half in double shear when compared to a single shear. Shear stresses are generally found in bolts, pins and rivets that are used to connect various structural members and machine components. 1.3.4 Bearing Stress: In the bolted connection in figure 1.5, a highly irregular pressure gets developed on the contact surface between the bolt and the plates. The average intensity of this pressure can be found out by dividing the load P by the projected area of the contact surface. This is referred to as the bearing stress.Indian Institute of Technology Madras
9. 9. Strength of Materials Prof. M. S. Sivakumar Figure 1.7 The projected area of the contact surface is calculated as the product of the diameter of the bolt and the thickness of the plate. Bearing stress, P P σb = = 1.5 A t×d Example 1: Figure 1.8Indian Institute of Technology Madras
10. 10. Strength of Materials Prof. M. S. Sivakumar A rod R is used to hold a sign board with an axial load 50 kN as shown in figure 1.8. The end of the rod is 50 mm wide and has a circular hole for fixing the pin which is 20 mm diameter. The load from the rod R is transferred to the base plate C through a bracket B that is 22mm wide and has a circular hole for the pin. The base plate is 10 mm thick and it is connected to the bracket by welding. The base plate C is fixed on to a structure by four bolts of each 12 mm diameter. Find the shear stress and bearing stress in the pin and in the bolts. Solution: Shear stress in the pin = τ pin V = = P = ( 50 × 103 / 2 )= 79.6 MPa A 2A π ( 0.02 )2 / 4 Force acting on the base plate = Pcosθ= 50 cos300 = 43.3 kN Shear stress in the bolt, τ bolt = P = ( ) 43.3 × 103 / 4 4A π ( 0.012 )2 / 4 = 95.7 MPa Bearing stress between pin and rod, σb = P = 50 × 103 ( ) b × d ( 0.05 ) × ( 0.02 ) = 50 MPa Bearing stress between pin and bracket = σb = P/2 = 50 × 103 / 2( ) b × d ( 0.022 ) × ( 0.02 ) = 56.8 MPa Bearing stress between plate and bolts = σb = P/4 = ( 43.3 × 103 / 4 ) t × d ( 0.01) × ( 0.012 ) = 90.2 MPa TopIndian Institute of Technology Madras
11. 11. Strength of Materials Prof. M. S. Sivakumar 1.4 Stress on inclined planes under axial loading: When a body is under an axial load, the plane normal to the axis contains only the normal stress as discussed in section 1.3.1. However, if we consider an oblique plane that forms an angle with normal plane, it consists shear stress in addition to normal stress. Consider such an oblique plane in a bar. The resultant force P acting on that plane will keep the bar in equilibrium against the external load P as shown in figure 1.9. Figure 1.9 The resultant force P on the oblique plane can be resolved into two components Fn and Fs that are acting normal and tangent to that plane, respectively. If A is the area of cross section of the bar, A/cos is the area of the oblique plane. Normal and shear stresses acting on that plane can be obtained as follows. Fn= Pcosθ Fs = -Psinθ (Assuming shear causing clockwise rotation negative). P cos θ P σ= = cos 2 θ 1.6 A / cos θ A P sin θ P τ=− = − sin θ cos θ 1.7 A / cos θ A Equations 1.6 and 1.7 define the normal and shear stress values on an inclined plane that makes an angle θ with the vertical plane on which the axial load acts. From above equations, it is understandable that the normal stress reaches its maximum when θ = 0o and becomes zero when θ = 90o.Indian Institute of Technology Madras
12. 12. Strength of Materials Prof. M. S. Sivakumar But, the shear stress assumes zero value at θ = 0o and θ = 90o and reaches its maximum when θ = 45o. The magnitude of maximum shear stress occurring at θ = 45o plane is half of the maximum normal stress that occurs at θ = 0o for a material under a uniaxial loading. P σ τmax = = max 1.8 2A 2 Now consider a cubic element A in the rod which is represented in two dimension as shown in figure 1.10 such that one of its sides makes an angle with the vertical plane. Figure 1.10 To determine the stresses acting on the plane mn, equations 1.6 and 1.7 are used as such and to knows the stresses on plane om, θ is replaced by θ + 90o. Maximum shear stress occurs on both om and mn planes with equal magnitude and opposite signs, when mn forms 45o angle with vertical plane. Example 2: A prismatic bar of sides 40 mm x 30 mm is axially loaded with a compressive force of 80 kN. Determine the stresses acting on an element which makes 300 inclination with the vertical plane. Also find the maximum shear stress value in the bar.Indian Institute of Technology Madras
13. 13. Strength of Materials Prof. M. S. Sivakumar Figure 1.11 Solution: Area of the cross section, A = 40 x 30 x 10-6 = 1.2 x 10-3 m2 P Normal stress on 300 inclined plane, σ = cos 2 θ A −80 × 103 = × cos 2 30o = −50 MPa −3 1.2 × 10 −P 80 × 103 Shear stress on 300 plane, τ = sin θ cos θ = × sin 300 × cos 300 −3 A 1.2 × 10 = 28.9 MPa [Counter clockwise] −80 × 103 Normal stress on 1200 plane, σ = cos 2 1200 = −16.67 MPa −3 1.2 × 10 80 × 103 Shear stress on 1200 plane, τ = × sin1200 × cos1200 = −28.9 MPa [Clock wise] −3 1.2 × 10 P 80 × 103 Maximum shear stress in the bar, τmax = = 2A 2 × 1.2 × 10−3 = ± 33.3 MPa TopIndian Institute of Technology Madras
14. 14. Strength of Materials Prof. M. S. Sivakumar 1.5 Strain The structural member and machine components undergo deformation as they are brought under loads. To ensure that the deformation is within the permissible limits and do not affect the performance of the members, a detailed study on the deformation assumes significance. A quantity called strain defines the deformation of the members and structures in a better way than the deformation itself and is an indication on the state of the material. Figure 1.12 Consider a rod of uniform cross section with initial length L0 as shown in figure 1.12. Application of a tensile load P at one end of the rod results in elongation of the rod by δ . After elongation, the length of the rod is L. As the cross section of the rod is uniform, it is appropriate to assume that the elongation is uniform throughout the volume of the rod. If the tensile load is replaced by a compressive load, then the deformation of the rod will be a contraction. The deformation per unit length of the rod along its axis is defined as the normal strain. It is denoted by ε δ L − L0 ε= = 1.9 L L Though the strain is a dimensionless quantity, units are often given in mm/mm, µm/m.Indian Institute of Technology Madras
15. 15. Strength of Materials Prof. M. S. Sivakumar Example 3: A circular hollow tube made of steel is used to support a compressive load of 500kN. The inner and outer diameters of the tube are 90mm and 130mm respectively and its length is 1000mm. Due to compressive load, the contraction of the rod is 0.5mm. Determine the compressive stress and strain in the post. Solution Force, P = −500 ×103 N (compressive) π Area of the tube, A = ⎡( 0.13) − ( 0.09 ) ⎤ = 6.912 × 10−3 m 2 2 2 4⎣⎢ ⎥ ⎦ P −500 × 103 Stress, σ = = = −72.3MPa (compressive) A 6.912 × 10−3 δ −0.5 Strain, ε = = = −5 × 10−4 (compressive) L0 1000 TopIndian Institute of Technology Madras
16. 16. Strength of Materials Prof. M. S. Sivakumar 1.6 Mechanical properties of materials A tensile test is generally conducted on a standard specimen to obtain the relationship between the stress and the strain which is an important characteristic of the material. In the test, the uniaxial load is applied to the specimen and increased gradually. The corresponding deformations are recorded throughout the loading. Stress-strain diagrams of materials vary widely depending upon whether the material is ductile or brittle in nature. If the material undergoes a large deformation before failure, it is referred to as ductile material or else brittle material. Figure 1.13 In figure 1.13, the stress-strain diagram of a structural steel, which is a ductile material, is given. Initial part of the loading indicates a linear relationship between stress and strain, and the deformation is completely recoverable in this region for both ductile and brittle materials. This linear relationship, i.e., stress is directly proportional to strain, is popularly known as Hookes law. σ = Eε 1.10 The co-efficient E is called the modulus of elasticity or Youngs modulus. Most of the engineering structures are designed to function within their linear elastic region only.Indian Institute of Technology Madras
17. 17. Strength of Materials Prof. M. S. Sivakumar After the stress reaches a critical value, the deformation becomes irrecoverable. The corresponding stress is called the yield stress or yield strength of the material beyond which the material is said to start yielding. In some of the ductile materials like low carbon steels, as the material reaches the yield strength it starts yielding continuously even though there is no increment in external load/stress. This flat curve in stress strain diagram is referred as perfectly plastic region. The load required to yield the material beyond its yield strength increases appreciably and this is referred to strain hardening of the material. In other ductile materials like aluminum alloys, the strain hardening occurs immediately after the linear elastic region without perfectly elastic region. After the stress in the specimen reaches a maximum value, called ultimate strength, upon further stretching, the diameter of the specimen starts decreasing fast due to local instability and this phenomenon is called necking. The load required for further elongation of the material in the necking region decreases with decrease in diameter and the stress value at which the material fails is called the breaking strength. In case of brittle materials like cast iron and concrete, the material experiences smaller deformation before rupture and there is no necking. Figure 1.14 TopIndian Institute of Technology Madras
18. 18. Strength of Materials Prof. M. S. Sivakumar 1.7 True stress and true strain In drawing the stress-strain diagram as shown in figure 1.13, the stress was calculated by dividing the load P by the initial cross section of the specimen. But it is clear that as the specimen elongates its diameter decreases and the decrease in cross section is apparent during necking phase. Hence, the actual stress which is obtained by dividing the load by the actual cross sectional area in the deformed specimen is different from that of the engineering stress that is obtained using undeformed cross sectional area as in equation 1.1 True stress or actual stress, P σact = 1.11 A act Though the difference between the true stress and the engineering stress is negligible for smaller loads, the former is always higher than the latter for larger loads. Similarly, if the initial length of the specimen is used to calculate the strain, it is called engineering strain as obtained in equation 1.9 But some engineering applications like metal forming process involve large deformations and they require actual or true strains that are obtained using the successive recorded lengths to calculate the strain. L dL ⎛ L ⎞ True strain = ∫ L = ln ⎜ ⎟ ⎝ L0 ⎠ 1.12 L0 True strain is also called as actual strain or natural strain and it plays an important role in theories of viscosity. The difference in using engineering stress-strain and the true stress-strain is noticeable after the proportional limit is crossed as shown in figure 1.15.Indian Institute of Technology Madras
19. 19. Strength of Materials Prof. M. S. Sivakumar Figure 1.15 TopIndian Institute of Technology Madras
20. 20. Strength of Materials Prof. M. S. Sivakumar 1.8 Poissons ratio Figure 1.16 Consider a rod under an axial tensile load P as shown in figure 1.6 such that the material P is within the elastic limit. The normal stress on x plane is σ xx = and the associated A σ longitudinal strain in the x direction can be found out from ε x = xx . As the material E elongates in the x direction due to the load P, it also contracts in the other two mutually perpendicular directions, i.e., y and z directions. Hence, despite the absence of normal stresses in y and z directions, strains do exist in those directions and they are called lateral strains. The ratio between the lateral strain and the axial/longitudinal strain for a given material is always a constant within the elastic limit and this constant is referred to as Poissons ratio. It is denoted by ν . lateral strain ν=− 1.13 axial strain Since the axial and lateral strains are opposite in sign, a negative sign is introduced in equation 1.13 to make ν positive. Using equation 1.13, the lateral strain in the material can be obtained by σ xx ε y = ε z = −νε x = −ν 1.14 E Poissons ratio can be as low as 0.1 for concrete and as high as 0.5 for rubber. In general, it varies from 0.25 to 0.35 and for steel it is about 0.3. TopIndian Institute of Technology Madras
22. 22. Strength of Materials Prof. M. S. Sivakumar Though the new elastic region CB resembles that of the initial elastic region OA, the internal structure of the material in the new state has changed. The change in the microstructure of the material is clear from the fact that the ductility of the material has come down due to strain hardening. When the material is reloaded, it follows the same path as that of a virgin material and fails on reaching the ultimate strength which remains unaltered due to the intermediate loading and unloading process. TopIndian Institute of Technology Madras
23. 23. Strength of Materials Prof. M. S. Sivakumar 1.10 Creep and fatigue In the preceding section, it was discussed that the plastic deformation of a material increases with increasing load once the stress in the material exceeds the elastic limit. However, the materials undergo additional plastic deformation with time even though the load on the material is unaltered. Consider a bar under a constant axial tensile load as shown in figure 1.18. Figure 1.18 As soon as the material is loaded beyond its elastic limit, it undergoes an instant plastic deformation ε 0 at time t = 0. Though the material is not brought under additional loads, it experiences further plastic deformation with time as shown in the graph in figure 1.18. This phenomenon is called creep. Creep at high temperature is of more concern and it plays an important role in the design of engines, turbines, furnaces, etc. However materials like concrete, steel and wood experience creep slightly even at normal room temperature that is negligible. Analogous to creep, the load required to keep the material under constant strain decreases with time and this phenomenon is referred to as stress relaxation. It was concluded in section 1.9 that the specimen will not fail when the stress in the material is with in the elastic limit.Indian Institute of Technology Madras
24. 24. Strength of Materials Prof. M. S. Sivakumar This holds true only for static loading conditions and if the applied load fluctuates or reverses then the material will fail far below its yield strength. This phenomenon is known as fatigue. Designs involving fluctuating loads like traffic in bridges, and reversing loads like automobile axles require fatigue analysis. Fatigue failure is initiated by a minute crack that develops at a high stress point which may be an imperfection in the material or a surface scratch. The crack enlarges and propagates through the material due to successive loadings until the material fails as the undamaged portion of the material is insufficient to withstand the load. Hence, a polished surface shaft can take more number of cycles than a shaft with rough or corroded surface. The number of cycles that can be taken up by a material before it fractures can be found out by conducting experiments on material specimens. The obtained results are plotted as σ − n curves as given in figure 1.19, which indicates the number of cycles that can be safely completed by the material under a given maximum stress. Figure 1.19 It is learnt from the graph that the number of cycles to failure increases with decrease in magnitude of stress.Indian Institute of Technology Madras
25. 25. Strength of Materials Prof. M. S. Sivakumar For steels, if the magnitude of stress is reduced to a particular value, it can undergo an infinitely large number of cycles without fatigue failure and the corresponding stress is known as endurance limit or fatigue limit. On the other hand, for non-ferrous metals like aluminum alloys there is no endurance limit, and hence, the maximum stress decreases continuously with increase in number of cycles. In such cases, the fatigue limit of the material is taken as the stress value that will allow an arbitrarily taken number of cycles, say 108 cycles. TopIndian Institute of Technology Madras
26. 26. Strength of Materials Prof. M. S. Sivakumar 1.11 Deformation in axially loaded members Consider the rod of uniform cross section under tensile load P along its axis as shown in figure 1.12. Let that the initial length of the rod be L and the deflection due to load be δ . Using equations 1.9 and 1.10, δ σ P =ε= = L E AE 1.15 PL δ= AE Equation 1.15 is obtained under the assumption that the material is homogeneous and has a uniform cross section. Now, consider another rod of varying cross section with the same axial load P as shown in figure 1.20. Figure 1.20 Let us take an infinitesimal element of length dx in the rod that undergoes a deflection dδ d δ due to load P. The strain in the element is ε = and dδ = εdx dx The deflection of total length of the rod can be obtained by integrating above equation, δ = ∫ εdx L Pdx δ= ∫ EA(x) 1.16 0Indian Institute of Technology Madras
27. 27. Strength of Materials Prof. M. S. Sivakumar As the cross sectional area of the rod keeps varying, it is expressed as a function of its length. If the load is also varying along the length like the weight of the material, it should also be expressed as a function of distance, i.e., P(x) in equation 1.16. Also, if the structure consists of several components of different materials, then the deflection of each component is determined and summed up to get the total deflection of the structure. When the cross section of the components and the axial loads on them are not varying along length, the total deflection of the structure can be determined easily by, n Pi Li δ=∑ 1.17 i =1 A i E i Example 4: Figure 1.21 Consider a rod ABC with aluminum part AB and steel part BC having diameters 25mm and 50 mm respectively as shown figure 1.21. Determine the deflections of points A and B.Indian Institute of Technology Madras
28. 28. Strength of Materials Prof. M. S. Sivakumar Solution: PAB L AB 10 × 103 × 400 Deflection of part AB = =− A AB E AB π × (0.025) 2 / 4 × 70 × 109 = −0.1164 mm PBC L BC 35 × 103 × 500 Deflection of part BC = =− A BC E BC π × (0.05) 2 / 4 × 200 × 109 = −0.0446 mm Deflection point of B = −0.0446 mm Deflection point of A = (−0.1164) + ( −0.0446 ) = −0.161mm TopIndian Institute of Technology Madras
29. 29. Strength of Materials Prof. M. S. Sivakumar 1.12 Statically indeterminate problems. Members for which reaction forces and internal forces can be found out from static equilibrium equations alone are called statically determinate members or structures. Problems requiring deformation equations in addition to static equilibrium equations to solve for unknown forces are called statically indeterminate problems. Figure 1.22 The reaction force at the support for the bar ABC in figure 1.22 can be determined considering equilibrium equation in the vertical direction. ∑ Fy = 0; R-P=0 Now, consider the right side bar MNO in figure 1.22 which is rigidly fixed at both the ends. From static equilibrium, we get only one equation with two unknown reaction forces R1 and R2. - P + R1 + R 2 = 0 1.18 Hence, this equilibrium equation should be supplemented with a deflection equation which was discussed in the preceding section to solve for unknowns. If the bar MNO is separated from its supports and applied the forces R1 ,R 2 and P , then these forces cause the bar to undergo a deflection δMO that must be equal to zero.Indian Institute of Technology Madras
30. 30. Strength of Materials Prof. M. S. Sivakumar δMO = 0 ⇒ δMN + δ NO = 0 1.19 δ MN and δ NO are the deflections of parts MN and NO respectively in the bar MNO. Individually these deflections are not zero, but their sum must make it to be zero. Equation 1.19 is called compatibility equation, which insists that the change in length of the bar must be compatible with the boundary conditions. Deflection of parts MN and NO due to load P can be obtained by assuming that the R1l1 R l material is within the elastic limit, δMN = and δ NO = 2 2 . A1E A2 E Substituting these deflections in equation 1.19, R1l1 R 2 l2 - =0 1.20 A1E A 2 E Combining equations 1.18 and 1.20, one can get, PA1l2 R1 = l1A 2 + l2 A1 1.21 PA 2 l1 R2 = l1A 2 + l2 A1 From these reaction forces, the stresses acting on any section in the bar can be easily determined. Example 5: Figure 1.23Indian Institute of Technology Madras
31. 31. Strength of Materials Prof. M. S. Sivakumar A rectangular column of sides 0.4m × 0.35m , made of concrete, is used to support a compressive load of 1.5MN. Four steel rods of each 24mm diameter are passing through the concrete as shown in figure 1.23. If the length of the column is 3m, determine the normal stress in the steel and the concrete. Take Esteel = 200 GPa and E concrete = 29 GPa. Solution: Ps = Load on each steel rod Pc = Load on concrete From equilibrium equation, Pc + 4Ps = P Pc + 4Ps = 1.5 × 103..........(a) Deflection in steel rod and concrete are the same. δconcrete = δsteel Pc × 3 Ps × 3 = ( 0.4 ) × (0.35) × 29 × 10 9 π × (0.024) 2 × 200 × 109 4 Pc = 44.87Ps ................(b) Combining equations (a) and (b), Ps = 30.7kN Pc = 1378kN P 1.378 × 106 Normal stress on concrete= c = = 9.84MPa Ac (0.4)(0.35) P 30.7 × 103 Normal stress on steel= s = = 67.86MPa As π 2 (0.024) 4 TopIndian Institute of Technology Madras
32. 32. Strength of Materials Prof. M. S. Sivakumar 1.13 Thermal effect When a material undergoes a change in temperature, it either elongates or contracts depending upon whether heat is added to or removed from the material. If the elongation or contraction is not restricted, then the material does not experience any stress despite the fact that it undergoes a strain. The strain due to temperature change is called thermal strain and is expressed as εT = α(∆T) 1.22 where αis a material property known as coefficient of thermal expansion and ∆T indicates the change in temperature. Since strain is a dimensionless quantity and ∆T is expressed in K or 0C, α has a unit that is reciprocal of K or 0C. The free expansion or contraction of materials, when restrained induces stress in the material and it is referred to as thermal stress. Thermal stress produces the same effect in the material similar to that of mechanical stress and it can be determined as follows. Figure 1.24 Consider a rod AB of length L which is fixed at both ends as shown in figure 1.24. Let the temperature of the rod be raised by ∆T and as the expansion is restricted, the material develops a compressive stress.Indian Institute of Technology Madras
33. 33. Strength of Materials Prof. M. S. Sivakumar In this problem, static equilibrium equations alone are not sufficient to solve for unknowns and hence is called statically indeterminate problem. To determine the stress due to ∆T, assume that the support at the end B is removed and the material is allowed to expand freely. Increase in the length of the rod δT due to free expansion can be found out using equation 1.22 δT = εT L = α (∆T)L 1.23 Now, apply a compressive load P at the end B to bring it back to its initial position and the deflection due to mechanical load from equation 1.15, PL δT = 1.24 AE As the magnitude of δT and δ are equal and their signs differ, δT = −δ PL α(∆T)L = − AE P Thermal stress, σT = = −α (∆T)E 1.25 A Minus sign in the equation indicates a compressive stress in the material and with decrease in temperature, the stress developed is tensile stress as ∆T becomes negative. It is to be noted that the equation 1.25 was obtained on the assumption that the material is homogeneous and the area of the cross section is uniform. Thermoplastic analysis assumes significance for structures and components that are experiencing high temperature variations.Indian Institute of Technology Madras
34. 34. Strength of Materials Prof. M. S. Sivakumar Example 6: Figure 1.25 A rod consists of two parts that are made of steel and aluminum as shown in figure 1.25. The elastic modulus and coefficient of thermal expansion for steel are 200GPa and 11.7 x 10-6 per 0C respectively and for aluminum 70GPa and 21.6 x 10-6 per 0C respectively. If the temperature of the rod is raised by 500C, determine the forces and stresses acting on the rod. Solution: Deflection of the rod under free expansion, δT = α(∆T)L ( ) ( = 11.7 × 10−6 × 50 × 500 + 21.6 × 10−6 × 50 × 750 ) = 1.1025 mm Restrained deflection of rod = 1.1025 - 0.4 = 0.7025 mm Let the force required to make their elongation vanish be R which is the reaction force at the ends.Indian Institute of Technology Madras
35. 35. Strength of Materials Prof. M. S. Sivakumar ⎛ RL ⎞ ⎛ RL ⎞ −δ = ⎜ ⎟ +⎜ ⎟ ⎝ AE ⎠steel ⎝ AE ⎠Al π Area of steel rod = [ 0.05] = 1.9635 × 10−3 m 2 2 4 π Area of aluminium rod = [ 0.03] = 0.7069 × 10−3 m 2 2 4 ⎡ 500 750 ⎤ −0.7025 = R ⎢ + ⎥ ⎣1.9635 × 10−3 × 200 × 109 0.7069 × 10−3 × 70 × 109 ⎦ Compressive force on the rod, R = − 42.076 kN P −42.76 × 103 Compressive stress on steel, σ = = = −21.8MPa A 1.9635 × 10−3 P −42.76 × 103 Compressive stress on steel, σ = = = −60.5MPa A 0.7069 × 10−3 TopIndian Institute of Technology Madras
36. 36. Strength of Materials Prof. M. S. Sivakumar 1.14. Design considerations: A good design of a structural element or machine component should ensure that the developed product will function safely and economically during its estimated life time. The stress developed in the material should always be less than the maximum stress it can withstand which is known as ultimate strength as discussed in section 1.6. During normal operating conditions, the stress experienced by the material is referred to as working stress or allowable stress or design stress. The ratio of ultimate strength to allowable stress is defined as factor of safety. Ultimate stress Factor of safety = 1.26 Allowable stress Factor of safety can also be expressed in terms of load as, Ultimate load Factor of safety = 1.27 Allowable load Equations 1.26 and 1.27 are identical when a linear relationship exists between the load and the stress. This is not true for many materials and equation 1.26 is widely used in design analysis. Factor of safety take care of the uncertainties in predicting the exact loadings, variation in material properties, environmental effects and the accuracy of methods of analysis. If the factor of safety is less, then the risk of failure is more and on the other hand, when the factor of safety is very high the structure becomes unacceptable or uncompetitive. Hence, depending upon the applications the factor of safety varies. It is common to see that the factor of safety is taken between 2 and 3. Stresses developed in the material when subjected to loads can be considered to be uniform at sections located far away from the point of application of loads. This observation is called Saint Venant’s principle and was discussed in section 1.3. But, when the element has holes, grooves, notches, key ways, threads and other abrupt changes in geometry, the stress on those cross-sections will not be uniform.Indian Institute of Technology Madras
37. 37. Strength of Materials Prof. M. S. Sivakumar These discontinuities in geometry cause high stresses concentrations in small regions of the material and are called stress raisers. Experimentally it was found that the stress concentrations are independent of the material size and its properties, and they depend only on the geometric parameters. Figure 1.26 Consider a rectangular flat plate with a circular hole as shown in figure 1.26. The stress distribution on the section passing through the centre of the hole indicates that the maximum stress occurs at the ends of the holes and it is much higher than the average stress. Since the designer, in general, is more interested in knowing the maximum stress rather than the actual stress distribution, a simple relationship between the σmax and σave in terms of geometric parameters will be of practical importance. Many experiments were conducted on samples with various discontinuities and the relationship between the stress concentration factor and the geometrical parameters are established, where σmax Stress concentration factor, K = 1.28 σaveIndian Institute of Technology Madras
38. 38. Strength of Materials Prof. M. S. Sivakumar P Hence, simply by calculating the average stress, σave = , in the critical section of a A discontinuity, σmax can be easily found and by multiplying σave with K. The variation of K in terms of r/d for the rectangular plate with a circular hole is given in figure 1.26. It is to be noted that the expression in equation 1.28 can be used as long as σmax is within the proportional limit of the material. Example 7: Figure 1.27 A rectangular link AB made of steel is used to support a load W through a rod CD as shown in figure 1.27. If the link AB is 30mm wide, determine its thickness for a factor of safety 2.5. The ultimate strength of steel may be assumed to be 450 MPa. Solution: Drawing free body diagram of the link and the rod, Taking moment about C,Indian Institute of Technology Madras
39. 39. Strength of Materials Prof. M. S. Sivakumar 25 × 550 − FBA sin 600 × 500 = 0 FBA = 31.75 kN Tension along link AB, FBA = 31.75 kN. Ultimate stress F.O.S = allowable stress 450 × 106 Allowable stress in link AB, σa = = 180 MPa 2.5 Tensile force Stress in link AB, σ = Area 31.75 × 103 180 ×106 = 0.03 × t Thickness of link AB, t = 5.88 t ≈ 6 mm TopIndian Institute of Technology Madras
40. 40. Strength of Materials Prof. M. S. Sivakumar 1.15. Strain energy: Strain energy is an important concept in mechanics and is used to study the response of materials and structures under static and dynamic loads. Within the elastic limit, the work done by the external forces on a material is stored as deformation or strain that is recoverable. On removal of load, the deformation or strain disappears and the stored energy is released. This recoverable energy stored in the material in the form of strain is called elastic strain energy. Figure 1.28 Consider a rod of uniform cross section with length L as shown in figure 1.28. An axial tensile load P is applied on the material gradually from zero to maximum magnitude and the corresponding maximum deformation is δ. Area under the load-displacement curve shown in figure 1.28 indicates the work done on the material by the external load that is stored as strain energy in the material. Let dW be the work done by the load P due to increment in deflection dδ. The corresponding increase in strain energy is dU. When the material is within the elastic limit, the work done due to dδ, dW = dU = Pdδ The total work done or total elastic strain energy of the material, δ W = U = ∫ Pdδ 1.29 0Indian Institute of Technology Madras
41. 41. Strength of Materials Prof. M. S. Sivakumar Equation 1.29 holds for both linear elastic and non-linear elastic materials. If the material is linear elastic, then the load-displacement diagram will become as shown in figure 1.29. Figure 1.29 The elastic strain energy stored in the material is determined from the area of triangle OAB. 1 U= P1δ1 1.30 2 P1L where δ1 = . AE Since the load-displacement curve is a straight line here, the load P1 can be expressed in terms of stiffness and deflection as P1 = kδ1 . Then equation 1.30 turns out to be, 1 U= kδ12 1.31 2 Work done and strain energy are expressed in N-m or joules (J). Strain energy defined in equation 1.29 depends on the material dimensions. In order to eliminate the material dimensions from the strain energy equation, strain energy density is often used. Strain energy stored per unit volume of the material is referred to as strain energy density. Dividing equation 1.29 by volume,Indian Institute of Technology Madras
42. 42. Strength of Materials Prof. M. S. Sivakumar ε Strain energy density, u = ∫ σdε 1.32 0 Equation 1.32 indicates the expression of strain energy in terms of stress and strain, which are more convenient quantities to use rather than load and displacement. Figure 1.30 Area under the stress strain curve indicates the strain energy density of the material. For linear elastic materials within proportional limit, equation 1.32 gets simplified as, 1 Strain energy density, u = σ1ε1 1.33 2 σ Using Hook’s law, ε1 = 1 , strain energy density is expressed in terms of stress, E σ12 u= 1.34 2E When the stress in the material reaches the yield stress σy , the strain energy density attains its maximum value and is called the modulus of resilience. σ 2 Modulus of resilience, u R = Y 1.35 2EIndian Institute of Technology Madras
43. 43. Strength of Materials Prof. M. S. Sivakumar Modulus of resilience is a measure of energy that can be absorbed by the material due to impact loading without undergoing any plastic deformation. Figure 1.31 If the material exceeds the elastic limit during loading, all the work done is not stored in the material as strain energy. This is due to the fact that part of the energy is spent on deforming the material permanently and that energy is dissipated out as heat. The area under the entire stress strain diagram is called modulus of toughness, which is a measure of energy that can be absorbed by the material due to impact loading before it fractures. Hence, materials with higher modulus of toughness are used to make components and structures that will be exposed to sudden and impact loads. Example 8: Figure 1.32Indian Institute of Technology Madras
44. 44. Strength of Materials Prof. M. S. Sivakumar A 25 kN load is applied gradually on a steel rod ABC as shown in figure 1.32. Taking E=200 GPa, determine the strain energy stored in the entire rod and the strain energy density in parts AB and BC. If the yield strength of the material is σy=320MPa, find the maximum energy that can be absorbed by the rod without undergoing permanent deformation. Solution: σ2 Strain energy density in part AB, u AB = AB 2E 2 ⎡ ⎤ 1 ⎢ 25 × 103 ⎥ u AB = ⎢ ⎥ 2 × 200 × 109 ⎢ π ( 0.024 )2 ⎥ ⎣4 ⎦ = 7.63 kJ/m3 σ2 Strain energy density in part BC, u BC = BC 2E 2 ⎡ ⎤ 1 ⎢ 25 × 103 ⎥ u BC = ⎢ ⎥ 2 × 200 × 109 ⎢ π ( 0.016 )2 ⎥ ⎣4 ⎦ = 38.65 kJ/m3 Strain energy in the entire rod, U = u ABVAB + u BC VBC ⎡Π ⎤ ⎡Π ⎤ = 7.63 ×103 × ⎢ ( 0.024 ) ×1⎥ + 38.65 ×103 × ⎢ ( 0.016 ) × 0.8⎥ 2 2 ⎣4 ⎦ ⎣4 ⎦ U = 9.67J The load that will produce yield stress in the material, Π P = σ y A BC = 320 × 106 × ( 0.016 )2 4 P = 64.3kN Maximum energy that can be stored in the rod,Indian Institute of Technology Madras
45. 45. Strength of Materials Prof. M. S. Sivakumar ⎡ 1 ⎢⎛ P ⎞ 2 ⎛ P ⎞ 2 ⎤ U= ⎜ ⎟ × VAB + ⎜ ⎟ × VBC ⎥ 2E ⎢⎝ A AB ⎠ ⎝ A BC ⎠ ⎥ ⎣ ⎦ P 2 ⎡ L AB L BC ⎤ = ⎢ + ⎥ 2E ⎣ A AB A BC ⎦ ( ⎡ ) ⎤ 2 64.3 ×103⎢ 1 0.8 ⎥ = ⎢Π + ⎥ 2 × 200 ×109 ⎢ ( 0.024 )2 Π ( 0.016 )2 ⎥ ⎣4 4 ⎦ = 63.97J TopIndian Institute of Technology Madras